264a1 complete handbook of sand casting part10
Post on 19-Dec-2015
Embed Size (px)
CORE NEEDED GREEN SAND CORE LEFT BY PAlTERN
Fig. 10-1. Examples of good and bad casting designs. (Continued from pages 160 and 161 .)
chaplets and that the print openings are sufficiently large enough to easily remove the core. (Core knock out.)
9. Avoid long slender cores through heavy metal sections or long spans. When unavoidable, they should be straight and well anchored to the mold.
10. Avoid metal inserts unless the section containing the insert is heavy enough to insure good purchase or the advantage gained by the use of inserts outweighs alternate steps.
11. Avoid the use of pattern letters on any surface other than one parallel to the parting.
12. Avoid sudden changes in section thicknesses creating hot spots.
13. Use ribs to stiffen or strengthen castings thus reducing weight.
14. Do not design a complicated casting in one piece, which would be much better produced as two or more castings welded or bolted together to give the desired results.
15. Do not try to cast sheet metal. Make a casting when the design dictates a casting, and go sheet metal when the design dictates it should be sheet metal.
16. Avoid all sharp comers and fillet all junctions. 17. Stagger crossing ribs so that the junction willnot form a hot
spot which could shrink. 18. If you can go any other way avoid deep pockets. If you
cannot, call for cover cores in place of green sand cores. 19. Design so that the casting can be easily poured and risers
are located a t the highest point in the mold for easy remov- al.
20. Avoid designing heavy sections which fall below light sec- tions in the mold that cannot be reached with risers. See Fig. 10-1.
ALTERNATE METHODS Before designing an item or part to be sand cast, you should
examine (if in your mind only) the possibility and feasability of producing it by any one of the many alternate methods of manufac- ture or fabrication, taking everything into consideration including cost. In other words you must make the decision based on many factors: Cost, quantity, weight, end use, product life, material, public acceptance etc. etc. (A broom should be made of straw not cast iron). There are many many items on the market today that are made of weldments, that should be castings and visa versa.
Ask yourself, sand casting or one of the following methods? Die casting Permanent mold Investment casting Shell (investment casting) Screw machine Stamping Weldment Forging Extrusion Header (hot or cold) Four slide Plastic injection EDM Sintered compact
If the answer is sand casting, you must then decide, based on metal, size, quantity, end use, cost etc., which way to go, green sand, dry sand, core mold, etc.
The point I am trying to make is you don't just up and design a Sand casting. There are many other things which should directly influence your design. They must all be taken into consideration. In one large (one of the Big Four) auto manufacturing plants, where I worked at one time, processing castings, we would make an isomet- ric drawing of the item or part, along with a positive of the interior and try in our mind to envision the patterns, core boxes, parting planes, flask equipment, gating, mold interior, casting, machining
and what have you before getting down to the actual designing. If it was not suited to sand casting we shipped it off to the division (forging etc.) where we thought it should be.
We have given the basic rules for sand casting design. If you cannot incorporate these rules with any degree of satisfaction into an intended casting design, perhaps what you have or want to make is not a casting.
Chapter 11 Casting Defects
A knowledge of casting defects is essential. If you cannot pinpoint the cause of a defect there is no way of correcting the problem. Some defects are quite obvious, along with the cause. Some types of defects can often resemble each other in appearance and separating them is often difficult A drawing or photograph of a defect is one thing and looking at the actual defect is another. You learn about defects by analyzing your own and those of others.
Here is a list of defects and their causes that should include anything you might ever encounter:
1. Poured short: Casting incomplete due to not filling the mold. This is a stupid trick which we all do-cause insuffi- cient metal in the ladle. Going back and touching up the mold will not do it.
2. Bobble: Here the casting will resemble a cold shut or that it was poured short. The problem was a slacked or inter- rupted pour. When pouring a casting the metal must be poured at a constant choked velocity. If you slack off or reduce the velocity, you can cause this defect. A com- pletely interrupted pour, start-stop-start, if only for a second. A great percentage of lost castings is caused by pouring improperly.
3. Slag inclusion: Slag on the face of the casting and usually down the sides of the sprue. The cause is not skimming the
ladle properly, not choking the sprue (keeping it brimming full from start to finish), sprue too big (cannot be kept choked) and gating system improperly choked.
4. S team gas porosity: This defect usually shows up as round holes like swiss cheese, just under the cope surface of the casting and comes to light during machining. The cause is a wet ladle, where the ladle lining was not properly and thoroughly dried. In extreme cases the metal will kick and boil in the ladle. The practice of pigging the metal in a wet ladle and refilling it with the hopes that the pigged metal finished drying the lade1 is sheer folly.
5. Kish: (cast iron) If the carbon equivalent of the iron is too high for the section poured and its cooling rate is slow, free graphite will form on the cope surface in black shiny flakes free from the casting, causing rough holey defects usually widespread. Carbon equivalent is the relationship of the total carbon, to the silicon and phosphorous content of the iron, which is controlled by the make up charge and silicon added at the spout. It is called carbon equivalent because the addition of silicon or phosphorus is only one third as effective as carbon, therefore the carbon equivalent of the three additives is equal to the total percentage of pure carbon plus one third the percentage of the silicon and phosphorus combined. The carbon equivalent is varied by the foundryman depending on what type of iron he is producing and what he is pouring.
6. Inverse Chill: This defect is found in gray iron castings and is hard or chilled iron in the center sandwiched bet- ween soft iron. The cause again could be incorrect carbon equivalent for the job or the presence of non-ferrous met- als in the charge, lead, antimony, tellurium which are detrimental impurities.
7. Broken Casting: This could be caused by improper de- sign. Improper filleting along with improper handling any where along the line. Copper base castings, red brass, yellow brass etc., are what are known as hot short, will break easily when hot. Thus, if the casting is shaken out of the mold before it has cooled sufficiently, it can get broken very easily. A mold or core which has too high a hot strength will not give or collapse to give the casting room to move as it shrinks and will break the casting.
8. Bleeder: This defect is caused by shaking the casting out too soon when a portion of it is still liquid. The section runs out leaving a defect. In extreme cases the entire center section will run out on the shake out man's feet.
9. Lead Sweat: A covering of lead tears on the outside of a high leaded bronze or brass casting with underlying holes or porosity (red metals containing a large Bercentage of lead such as leaded bearing bronze). Since the lead has the lowest melting point of the constituents of high leaded bronze (copper 70 percent-tin 5 percent-lead 25 per- cent) and is not in solution with the copper and tin, it remains liquid until the casting has cooled below 620 de- grees Fahrenheit. If the casting is shaken out before it is below this temperature the lead will sweat out &om bet- ween the copper and tin crystals.
10. Run Out: This is caused by the metal in the mold running out between the joint of the flask, which drains the liquid metal partially or completely from any portion of the cast- ing above the parting line. A run out can come through or between the drag and the bottom board from a cracked drag mold. Also, it can come from between a loose impro- perly fitting core and the core print. It is caused by insuffi- cient room between the flask and the cavity, insufficient weight on the cope (cope raises during pouring) or impro- perly clamped molds. Excessive hydrostatic pressure (sprue too tall for the job) no dough roll used between cope and drag (large jobs) or a combination of all of the above.
An attempt to save a run out by placing your foot on top of the cope and applying pressure above the point. where the liquid metal is running out is foolhardy and dangerous. Also trying to stop off the run out flow with sand or clay is folly.
11. Omission of a core: Results and cause obvious. I 12. Ram Off: I s a defect resulting from a section of the mold
being forced away from the pattern by ramming sand after it has conformed to the pattern contour. This is caused by careless ramming where the mold is rammed vertically and then on an angle, causing the vertically rammed sand to slide sideways leaving a gap between the pattern and the sand, resulting in a deformed casting. Another cause is using a sand with poor or low flowabiity. (Too much clay or sand too h e . )
13. Core Rise: This defect is caused by a core rising from its intended position toward the cope surface, causing